I COUPLED SIMULATIONS OF MECHANICAL ... /67531/metadc687477/... strain rate dependent such that z is
Embed Size (px)
Transcript of I COUPLED SIMULATIONS OF MECHANICAL ... /67531/metadc687477/... strain rate dependent such that z is
COUPLED SIMULATIONS OF MECHANICAL DEFORMATION AND MICROSTRUCTURAL EVOLUTION USING
POLYCRYSTAL PLASTICITY AND MONTE CARLO POTTS MODELS
C.C. BATTAILE, T.E. BUCHHEIT, E.A. HOLM, G.W. WELLMAN, AND M.K. NEILSEN Sandia National Laboratories, Albuquerque, NM 87185-141 1, email@example.com
The microstructural evolution of heavily deformed polycrystalline Cu is simulated by coupling a constitutive model for polycrystal plasticity with the Monte Carlo Potts model for grain growth. The effects of deformation on boundary topology and grain growth kinetics are presented. Heavy deformation leads to dramatic strain-induced boundary migration and subsequent grain fra,omentation. Grain growth is accelerated in heavily deformed microstructures. The implications of these results for the thermomechanical fatigue failure of eutectic solder joints are discussed.
Thermal fluctuations during the normal course of service or storage can accelerate the failure of solder joints in electronic components [l]. This thermomechanical fatigue 0 of solder joints involves a number of different processes acting in concert. Thermal expansions and contractions of the surrounding pieces generate a complex state of stress in the joint. The local details of that stress state, and the properties of the solder microstructure, create regions of high localized strain in the joint. These localized deformations induce coarsening in the microstructure, which weakens the material. These weakened regions fatigue as the thermal fluctuations continue, eventually leading to component failure. This phenomenon has been observed, for example, as satellites pass into and out of the sun’s rays, or when stored components are subjected to daily and seasonal temperature changes.
Understanding TMF requires an examination of how each process operates individually and in conjunction with the other processes. In this paper, we examine the effects of the localized deformation on the evolution of a polycrystal microstructure. Solder joints are typically composed of eutectic PbSn, but we will use pure polycrystalline Cu as a proof-of-concept system for the present study. The deformation of the material is simulated using the finite element method ( E M ) with a constitutive law for polycrystal plasticity fit to experimental data for Cu. This polycrystal plasticity model predicts the local mechanical state of the system, and this information is combined with the Monte Carlo Potts model to simulate grain growth (Le., microstructural coarsening) in the deformed material. The polycrystal plasticity and Potts models will be outlined briefly, and the extension of the Potts model to account for stored strain energies will be discussed. The effects of deformation on the evolution of the microstructure will be presented, and the implications of these results for the TMF of solder joints will be addressed.
The polycrystal plasticity model will be described here only in brief, and the reader is referred elsewhere [2,3] for a more detailed discussion. The local states of stress and strain in the Cu polycrystal are simulated using FEM with a constitutive law for polycrystal plasticity fit to experimental data for Cu. The finite element mesh is generated by discretizing a polycrystal microstructure onto a cubic lattice. Each lattice site is associated with a spatial orientation, and a cluster of lattice sites with the same orientation represents a grain. Each lattice site represents an element in the finite element mesh, and the nodes of the mesh form a cubic grid occupying the comers of the elements. Ideally, the polycrystal microstructure would correspond directly to the real Cu sample to which the plasticity model was fit. However, for the purpose of the present study, the microstructure was taken from a conventional 3D Potts model simulation, and the
This report was prepared as an account of work sponsored by an agency of the United States Government. Neither the United States Government nor any agency thereof, nor any of their employees, make any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness, or usefulness of any information, apparatus, product, or process disclosed, or represents that its use would not infringe privately owned rights. Reference herein to any specific commercial product, process, or service by trade name, trademark, manufacturer, or otherwise does not necessarily constitute or imply its endorsement, recommendation, or favoring by the United States Government or any agency thereof. The views and opinions of authors expressed herein do not necessarily state or reflect those of the United States Government or any agency thereof.
Portions of this document may be illegible in electronic image products. Images are produced from the best available original document.
orientations of the grains are assigned at random.
orientations of the material at each element, and the material deformations on each of the twelve FCC slip systems. The elastic response of the material is anisotropic, and the plastic response is strain rate dependent such that z is the strain rate sensitivity exponent. In this study, an exponent of m = 10 was used. Each of the twelve slip systems hardens isotropically according to a power law,
The constitutive model for the mechanical response of a polycrystal tracks the spatial
y", where zis the shear stress, f is the shear strain rate, and rn
where Z, is the initial critical resolved shear stress, yis the effective plastic shear strain, and A and n are parameters fit to the experimental stress-strain response of a Cu polycrystal. All slip systems are initialized to the same critical resolved shear stress and harden equally. However, the polycrystal evolves an anisotropic mechanical response during deformation due to the variations in geometric constraints between and within grains.
The plasticity simulation is performed on a 54-grain polycrystal microstructure mapped onto a 30x30x30-element mesh. The average grain size is about 500 elements. Each element is cubic before deformation. The initial element orientations in each grain are the same (random) value, and the stress and strain values at each element set to zero. Periodic boundary conditions are imposed in all three directions. Deformation is simulated by a prescribed elongation of the simulation cell in one direction, with zero net force in the other two directions. The elongation of the simulation cell is increased in increments of 0.00 1 %. At each strain increment, the mechanical state of the system is equilibrated. The stress and strain increments on each slip system in each element are used to calculate the stored plastic energy, which is input to a Monte Carlo Potts model of microstructure evolution, as described below. (Stored elastic energy is relatively small at the deformations of interest, and is therefore neglected in the present study, though it may be important under certain circumstances.)
The evolution of the deformed microstructures is simulated using a Monte Carlo Potts model [4,5] modified to account for the plastic energy stored in the material during deformation. The finite element mesh is input directly to the Potts simulation. Each grain on the mesh is assigned a unique integer identity, or "spin," and all the elements in a grain assume the spin of that grain. Periodic boundary conditions are imposed in all directions. Each element contains twelve slip systems for which the twelve shear stress and strain increments are taken from the polycrystal plasticity model.
The system energy is described by a modified Potts Hamiltonian,
The sum over i includes all of the N elements in the mesh, and the sum overj includes all of the 26 elements that share at least one node with element i. (Recall that the mesh is initially cubic, and thus the element connectivity of the deformed mesh is that of a cubic grid.) The sum over AZ includes all elongation increments up to the elongation of interest, A$, and the sum over a includes all twelve slip systems in element i. E, is a measure of the grain boundary energy, and is assumed to be unity for all boundaries in this study. si is the spin of element i, and 6(s,,sj) is the Kronecker delta, i.e., 6(si,sj) = 1 if si = sj and 0 otherwise. v. is the volume of element i, z, is the initial critical resolved shear stress, z,(a,AZ) is the average plastic shear stress on slip system a in element i at elongation AZ, and Ax(a,AZ) is the plastic shear strain increment on slip system a in element i at elongation AZ. The first term in Equ. 2 represents the grain boundary energy, and the second describes the stored plastic energy.
The lMonte Carlo Potts simulation proceeds by choosing an element at random and attempting to change its spin to that of one of its neighbors. When an element changes its spin to
that of a different grain, the stored plastic energy in that element is changed to the average of the values at the neighboring elements that belong to that different grain. This implies that, when a grain boundary moves, nearly all of the dislocations adjacent to the boundary are extended into the material through which the boundary migrates. However, this is not always the case in reality. On the other hand, if no dislocations were propagated with the boundary, then a new grain would be introduced and the material would